Ultrastable, cationic three-dimensional lead bromide frameworks that intrinsically emit broadband white-light.
Peng, Chengdong; Zhuang, Zewen; Yang, Huimin; Zhang, Guiyang; Fei, Honghan; Chemical science 9 (2018) 1627–1633; doi:10.1039/c7sc04118g

data_1548493
_publ_section_title
;
 Ultrastable, cationic three-dimensional lead bromide frameworks that
 intrinsically emit broadband white-light.
;
_journal_issue                   6
_journal_name_full               'Chemical science'
_journal_page_first              1627
_journal_page_last               1633
_journal_paper_doi               10.1039/c7sc04118g
_journal_volume                  9
_journal_year                    2018
_chemical_formula_moiety         'C3 H4 Br Cl0 O2 Pb'
_chemical_formula_sum            'C3 H4 Br Cl0 O2 Pb'
_chemical_formula_weight         359.16
_space_group_IT_number           92
_space_group_name_Hall           'P 4abw 2nw'
_space_group_name_H-M_alt        'P 41 21 2'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  'P 4abw 2nw'
_symmetry_space_group_name_H-M   'P 41 21 2'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2017-09-20 deposited with the CCDC.
2017-12-19 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   9.0035(13)
_cell_length_b                   9.0035(13)
_cell_length_c                   14.390(2)
_cell_measurement_reflns_used    9872
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      27.47
_cell_measurement_theta_min      3.20
_cell_volume                     1166.5(3)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1545
_diffrn_reflns_av_sigmaI/netI    0.0516
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            12812
_diffrn_reflns_theta_full        24.99
_diffrn_reflns_theta_max         24.99
_diffrn_reflns_theta_min         4.74
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    35.663
_exptl_absorpt_correction_T_max  0.0696
_exptl_absorpt_correction_T_min  0.0217
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            clear
_exptl_crystal_density_diffrn    4.090
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       bulk
_exptl_crystal_F_000             1240
_exptl_crystal_size_max          0.46
_exptl_crystal_size_mid          0.33
_exptl_crystal_size_min          0.16
_refine_diff_density_max         3.157
_refine_diff_density_min         -2.664
_refine_diff_density_rms         0.465
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.08(5)
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.053
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     45
_refine_ls_number_reflns         1026
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.053
_refine_ls_R_factor_all          0.0601
_refine_ls_R_factor_gt           0.0588
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1078P)^2^+16.6752P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1522
_refine_ls_wR_factor_ref         0.1537
_reflns_number_gt                993
_reflns_number_total             1026
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c7sc04118g2.cif
_cod_data_source_block           mo_170410a
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Tetragonal' changed to 'tetragonal'
according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 

 Adding full bibliography for 1548493--1548495.cif.
;
_cod_database_code               1548493